Constitutive Equations


 Augusta Harrell
 1 years ago
 Views:
Transcription
1 Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module 8), equilibrium (Module 9), and tensor transformations (Module 0) contain concepts vital to Mechanics of Materials, but they do not provide insight on the role of the material itself. The kinematic equations relate strains to displacement gradients, and the equilibrium equations relate stress to the applied tractions on loaded boundaries and also govern the relations among stress gradients within the material. In three dimensions there are six kinematic equations and three equilibrum equations, for a total of nine. However, there are fifteen variables: three displacements, six strains, and six stresses. We need six more equations, and these are provided by the material s consitutive relations: six expressions relating the stresses to the strains. These are a sort of mechanical equation of state, and describe how the material is constituted mechanically. With these constitutive relations, the vital role of the material is reasserted: The elastic constants that appear in this module are material properties, subject to control by processing and microstructural modification as outlined in Module 2. This is an important tool for the engineer, and points up the necessity of considering design of the material as well as with the material. Isotropic elastic materials In the general case of a linear relation between components of the strain and stress tensors, we might propose a statement of the form ɛ ij = S ijkl σ kl where the S ijkl is a fourthrank tensor. This constitutes a sequence of nine equations, since each component of ɛ ij is a linear combination of all the components of σ ij. For instance: ɛ 23 = S 23 σ + S 232 σ 2 + +S 2333 ɛ 33 Based on each of the indices of S ijkl taking on values from to 3, we might expect a total of 8 independent components in S. However, both ɛ ij and σ ij are symmetric, with six rather than nine independent components each. This reduces the number of S components to 36, as can be seen from a linear relation between the pseudovector forms of the strain and stress:
2 ɛ x S S 2 S 6 ɛ z S 2 S 22 S 26 = γ. yz..... γ xz S 6 S 26 S 66 γ xy It can be shown that the S matrix in this form is also symmetric. It therefore it contains only 2 independent elements, as can be seen by counting the elements in the upper right triangle of the matrix, including the diagonal elements ( = 2). If the material exhibits symmetry in its elastic response, the number of independent elements in the S matrix can be reduced still further. In the simplest case of an isotropic material, whose stiffnesses are the same in all directions, only two elements are independent. We have earlier shown that in two dimensions the relations between strains and stresses in isotropic materials can be written as σ x σ y σ z τ yz τxz τ xy () ɛ x = (σ x νσ y ) = (σ y νσ x ) γ xy = G τ xy (2) along with the relation G = 2( + ν) xtending this to three dimensions, the pseudovectormatrix form of qn. for isotropic materials is ɛ x ɛ z γ yz γ xz γ xy = G G G The quantity in brackets is called the compliance matrix of the material, denoted S or S ij. It is important to grasp the physical significance of its various terms. Directly from the rules of matrix multiplication, the element in the i th row and j th column of S ij is the contribution of the j th stress to the i th strain. For instance the component in the,2 position is the contribution of the ydirection stress to the xdirection strain: multiplying σ y by / gives the ydirection strain generated by σ y, and then multiplying this by gives the Poisson strain induced in the x direction. The zero elements show the lack of coupling between the normal and shearing components. The isotropic constitutive law can also be written using index notation as (see Prob. ) ɛ ij = +ν σ ij ν δ ijσ kk (4) where here the indicial form of strain is used and G has been eliminated using G = /2( + ν) The symbol δ ij is the Kroenecker delta, described in the Module on Matrix and Index Notation. σ x σ y σ z τ yz τxz τ xy G.M. Mase, Schaum s Outline of Theory and Problems of Continuum Mechanics, McGrawHill, (3)
3 If we wish to write the stresses in terms of the strains, qns. 3 can be inverted. In cases of plane stress (σ z = τ xz = τ yz = 0), this yields σ x σ y τ xy = ν 2 ν 0 ν ()/2 ɛ x γ xy where again G has been replaced by /2( + ν). Or, in abbreviated notation: where D = S is the stiffness matrix. Hydrostatic and distortional components (5) σ = Dɛ (6) Figure : Hydrostatic compression. A state of hydrostatic compression, depicted in Fig., is one in which no shear stresses exist and where all the normal stresses are equal to the hydrostatic pressure: σ x = σ y = σ z = p where the minus sign indicates that compression is conventionally positive for pressure but negative for stress. For this stress state it is obviously true that 3 (σ x + σ y + σ z )= 3 σ kk = p so that the hydrostatic pressure is the negative mean normal stress. This quantity is just one third of the stress invariant I, which is a reflection of hydrostatic pressure being the same in all directions, not varying with axis rotations. In many cases other than direct hydrostatic compression, it is still convenient to dissociate the hydrostatic (or dilatational ) component from the stress tensor: σ ij = 3 σ kkδ ij +Σ ij (7) Here Σ ij is what is left over from σ ij after the hydrostatic component is subtracted. The Σ ij tensor can be shown to represent a state of pure shear, i.e. there exists an axis transformation such that all normal stresses vanish (see Prob. 5). The Σ ij is called the distortional, or deviatoric, 3
4 component of the stress. Hence all stress states can be thought of as having two components as shown in Fig. 2, one purely extensional and one purely distortional. This concept is convenient because the material responds to these stress components is very different ways. For instance, plastic and viscous flow is driven dominantly by distortional components, with the hydrostatic component causing only elastic deformation. Figure 2: Dilatational and deviatoric components of the stress tensor. Consider the stress state σ = xample , GPa The mean normal stress is σ kk /3=(5+8+2)/3 = 5, so the stress decomposition is σ = σ kkδ ij +Σ ij = It is not obvious that the deviatoric component given in the second matrix represents pure shear, since there are nonzero components on its diagonal. However, a stress transformation using uler angles ψ = φ =0,θ = 9.22 gives the stress state Σ = The hydrostatic component of stress is related to the volumetric strain through the modulus of compressibility ( p = K V/V), so 3 σ kk = Kɛ kk (8) Similarly to the stress, the strain can also be dissociated as ɛ ij = 3 ɛ kkδ ij + e ij where e ij is the deviatoric component of strain. The deviatoric components of stress and strain are related by the material s shear modulus: Σ ij =2Ge ij (9) 4
5 where the factor 2 is needed because tensor descriptions of strain are half the classical strains for which values of G have been tabulated. Writing the constitutive equations in the form of qns. 8 and 9 produces a simple form without the coupling terms in the conventional ν form. xample 2 Using the stress state of the previous example along with the elastic constants for steel ( = 207 GPa,ν = 0.3,K = /3( 2ν) = 73 GPa,G = /2( + ν) = 79.6 Gpa), the dilatational and distortional components of strain are δ ij ɛ kk = δ ijσ kk 3K = e ij = Σ ij 2G = The total strain is then ɛ ij = 3 ɛ kkδ ij + e ij = If we evaluate the total strain using qn. 4, we have ɛ ij = +ν σ ij ν δ ijσ kk = These results are the same, differing only by roundoff error. Finite strain model When deformations become large, geometrical as well as material nonlinearities can arise that are important in many practical problems. In these cases the analyst must employ not only a different strain measure, such as the Lagrangian strain described in Module 8, but also different stress measures (the Second PiolaKirchoff stress replaces the Cauchy stress when Lagrangian strain is used) and different stressstrain constitutive laws as well. A treatment of these formulations is beyond the scope of these modules, but a simple nonlinear stressstrain model for rubbery materials will be outlined here to illustrate some aspects of finite strain analysis. The text by Bathe 2 provides a more extensive discussion of this area, including finite element implementations. In the case of small displacements, the strain ɛ x is given by the expression: ɛ x = [σ x ν(σ y + σ z )] For the case of elastomers with ν =0.5, this can be rewritten in terms of the mean stress σ m =(σ x +σ y +σ z )/3as: 2ɛ x = 3 (σ x σ m ) 2 K.J. Bathe, Finite lement Procedures in ngineering Analysis, PrenticeHall,
6 For the largestrain case, the following analogous stressstrain relation has been proposed: λ 2 x =+2ɛ x= 3 (σ x σ m ) (0) where here ɛ x is the Lagrangian strain and σ m is a parameter not necessarily equal to σ m. The σ m parameter can be found for the case of uniaxial tension by considering the transverse contractions λ y = λ z : λ 2 y = 3 (σ y σ m) Since for rubber λ x λ y λ z =,λ 2 y =/λ x. Making this substitution and solving for σ m : Substituting this back into qn. 0, Solving for σ x, σ m = λ2 y 3 λ 2 x = 3 = 3λ x [ σ x ] 3λ x (λ 2x λx ) σ x = 3 Here the stress σ x = F/A is the true stress based on the actual (contracted) crosssectional area. The engineering stress σ e = F/A 0 based on the original area A 0 = Aλ x is: σ e = σ ( x = G λ x ) λ x λ 2 x where G = /2( + ν) =/3 forν=/2. This result is the same as that obtained in Module 2 by considering the force arising from the reduced entropy as molecular segments spanning crosslink sites are extended. It appears here from a simple hypothesis of stressstrain response, using a suitable measure of finite strain. Anisotropic materials Figure 3: An orthotropic material. If the material has a texture like wood or unidirectionallyreinforced fiber composites as shown in Fig. 3, the modulus in the fiber direction will typically be larger than those in the transverse directions ( 2 and 3 ). When 2 3, the material is said to be orthotropic. 6
7 It is common, however, for the properties in the plane transverse to the fiber direction to be isotropic to a good approximation ( 2 = 3 ); such a material is called transversely isotropic. The elastic constitutive laws must be modified to account for this anisotropy, and the following form is an extension of qn. 3 for transversely isotropic materials: ɛ ɛ 2 γ 2 = / 2 / / / /G 2 The parameter ν 2 is the principal Poisson s ratio; it is the ratio of the strain induced in the 2direction by a strain applied in the direction. This parameter is not limited to values less than 0.5 as in isotropic materials. Conversely, ν 2 gives the strain induced in the direction by a strain applied in the 2direction. Since the 2direction (transverse to the fibers) usually has much less stiffness than the direction, it should be clear that a given strain in the direction will usually develop a much larger strain in the 2direction than will the same strain in the 2direction induce a strain in the direction. Hence we will usually have ν 2 >ν 2. There are five constants in the above equation (, 2, ν 2, ν 2 and G 2 ). However, only four of them are independent; since the S matrix is symmetric, ν 2 / 2 = ν 2 /. A table of elastic constants and other properties for widely used anisotropic materials can be found in the Module on Composite Ply Properties. The simple form of qn., with zeroes in the terms representing coupling between normal and shearing components, is obtained only when the axes are aligned along the principal material directions; i.e. along and transverse to the fiber axes. If the axes are oriented along some other direction, all terms of the compliance matrix will be populated, and the symmetry of the material will not be evident. If for instance the fiber direction is offaxis from the loading direction, the material will develop shear strain as the fibers try to orient along the loading direction as shown in Fig. 4. There will therefore be a coupling between a normal stress and a shearing strain, which never occurs in an isotropic material. σ σ 2 τ 2 () Figure 4: Shearnormal coupling. The transformation law for compliance can be developed from the transformation laws for strains and stresses, using the procedures described in Module 0 (Transformations). By successive transformations, the pseudovector form for strain in an arbitrary xy direction shown in Fig. 5 is related to strain in the 2 (principal material) directions, then to the stresses in the 2 directions, and finally to the stresses in the xy directions. The final grouping of transformation matrices relating the xy strains to the xy stresses is then the transformed compliance matrix 7
8 Figure 5: Axis transformation for constitutive equations. in the xy direction: ɛ x ɛ x ɛ γ = R xy 2 γ = RA ɛ 2 xy 2 γ = RA R 2 σ σ x = RA R S σ 2 τ = RA R SA σ y 2 τ S xy where S is the transformed compliance matrix relative to xy axes. Here A is the transformation matrix, and R is the Reuter s matrix defined in the Module on Tensor Transformations. The inverse of S is D, the stiffness matrix relative to xy axes: σ x σ y τ xy S = RA R SA, D = S (2) ɛ ɛ 2 γ 2 xample 3 Consider a ply of Kevlarepoxy composite with a stiffnesses = 82, 2 =4,G 2 =2.8(allGPa)and ν 2 =0.25. The compliance matrix S in the 2 (material) direction is: S = / 2 / / / /G 2 = If the ply is oriented with the fiber direction (the direction) at θ =30 from the xy axes, the appropriate transformation matrix is A = c2 s 2 s c 2 2sc 2sc = sc sc c 2 s The compliance matrix relative to the xy axes is then S = RA R SA = Note that this matrix is symmetric (to within numerical roundoff error), but that nonzero coupling values exist. A user not aware of the internal composition of the material would consider it completely anisotropic. 8
9 The apparent engineering constants that would be observed if the ply were tested in the xy rather than 2 directions can be found directly from the trasnformed S matrix. For instance, the apparent elastic modulus in the x direction is x =/S, =/( )=.33 GPa. Problems. xpand the indicial forms of the governing equations for solid elasticity in three dimensions: equilibrium : σ ij,j =0 kinematic : ɛ ij =(u i,j + u j,i )/2 constitutive : ɛ ij = +ν σ ij ν δ ijσ kk + αδ ij T where α is the coefficient of linear thermal expansion and T is a temperature change. 2. (a) Write out the compliance matrix S of qn. 3 for polycarbonate using data in the Module on Material Properties. (b) Use matrix inversion to obtain the stiffness matrix D. (c) Use matrix multiplication to obtain the stresses needed to induce the strains ɛ = ɛ x ɛ z γ yz γ xz γ xy = (a) Write out the compliance matrix S of qn.3 for an aluminum alloy using data in the Module on Material Properties. (b) Use matrix inversion to obtan the stiffness matrix D. (c) Use matrix multiplication to obtain the stresses needed to induce the strains 4. Given the stress tensor ɛ = ɛ x ɛ z γ yz γ xz γ xy = σ ij = (MPa) (a) Dissociate σ ij into deviatoric and dilatational parts Σ ij and (/3)σ kk δ ij. 9
10 (b) Given G = 357 MPa and K =.67 GPa, obtain the deviatoric and dilatational strain tensors e ij and (/3)ɛ kk δ ij. (c) Add the deviatoric and dilatational strain components obtained above to obtain the total strain tensor ɛ ij. (d) Compute the strain tensor ɛ ij using the alternate form of the elastic constitutive law for isotropic elastic solids: ɛ ij = +ν σ ij ν δ ijσ kk Compare the result with that obtained in (c). 5. Provide an argument that any stress matrix having a zero trace can be transformed to one having only zeroes on its diagonal; i.e. the deviatoric stress tensor Σ ij represents a state of pure shear. 6. Write out the xy twodimensional compliance matrix S and stiffness matrix D (qn. 2) for a single ply of graphite/epoxy composite with its fibers aligned along the x axes. 7. Write out the xy twodimensional compliance matrix S and stiffness matrix D (qn. 2) for a single ply of graphite/epoxy composite with its fibers aligned 30 from the x axis. 0
Understand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationThe Kinematic Equations
The Kinematic Equations David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 0139 September 19, 000 Introduction The kinematic or straindisplacement
More informationA short review of continuum mechanics
A short review of continuum mechanics Professor Anette M. Karlsson, Department of Mechanical ngineering, UD September, 006 This is a short and arbitrary review of continuum mechanics. Most of this material
More information16.21 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive Equations
6.2 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive quations Constitutive quations For elastic materials: If the relation is linear: Û σ ij = σ ij (ɛ) = ρ () ɛ ij σ ij =
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationConstitutive Relations
Constitutive Relations Dr. Andri Andriyana Centre de Mise en Forme des Matériaux, CEMEF UMR CNRS 7635 École des Mines de Paris, 06904 Sophia Antipolis, France Spring, 2008 Outline Outline 1 Review of field
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationConstitutive Relations
Constitutive Relations Andri Andriyana, Ph.D. Centre de Mise en Forme des Matériaux, CEMEF UMR CNRS 7635 École des Mines de Paris, 06904 Sophia Antipolis, France Spring, 2008 Outline Outline 1 Review of
More informationPEAT SEISMOLOGY Lecture 2: Continuum mechanics
PEAT8002  SEISMOLOGY Lecture 2: Continuum mechanics Nick Rawlinson Research School of Earth Sciences Australian National University Strain Strain is the formal description of the change in shape of a
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More information3.22 Mechanical Properties of Materials Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 3.22 Mechanical Properties of Materials Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Quiz #1 Example
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationChapter 2: Elasticity
OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.
More informationChapter 1. Continuum mechanics review. 1.1 Definitions and nomenclature
Chapter 1 Continuum mechanics review We will assume some familiarity with continuum mechanics as discussed in the context of an introductory geodynamics course; a good reference for such problems is Turcotte
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More information3.2 Hooke s law anisotropic elasticity Robert Hooke ( ) Most general relationship
3.2 Hooke s law anisotropic elasticity Robert Hooke (16351703) Most general relationship σ = C ε + C ε + C ε + C γ + C γ + C γ 11 12 yy 13 zz 14 xy 15 xz 16 yz σ = C ε + C ε + C ε + C γ + C γ + C γ yy
More informationHÅLLFASTHETSLÄRA, LTH Examination in computational materials modeling
HÅLLFASTHETSLÄRA, LTH Examination in computational materials modeling TID: 20162810, kl 14.0019.00 Maximalt 60 poäng kan erhållas på denna tenta. För godkänt krävs 30 poäng. Tillåtet hjälpmedel: räknare
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationMATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS
. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stressstrain
More informationUseful Formulae ( )
Appendix A Useful Formulae (985989993) 34 Jeremić et al. A.. CHAPTER SUMMARY AND HIGHLIGHTS page: 35 of 536 A. Chapter Summary and Highlights A. Stress and Strain This section reviews small deformation
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam
MODELING OF CONCRETE MATERIALS AND STRUCTURES Class Meeting #1: Fundamentals Kaspar Willam University of Colorado at Boulder Notation: Direct and indicial tensor formulations Fundamentals: Stress and Strain
More information2.2 Relation Between Mathematical & Engineering Constants Isotropic Materials Orthotropic Materials
Chapter : lastic Constitutive quations of a Laminate.0 Introduction quations of Motion Symmetric of Stresses Tensorial and ngineering Strains Symmetry of Constitutive quations. ThreeDimensional Constitutive
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More informationContinuum Mechanics and the Finite Element Method
Continuum Mechanics and the Finite Element Method 1 Assignment 2 Due on March 2 nd @ midnight 2 Suppose you want to simulate this The familiar massspring system l 0 l y i X y i x Spring length before/after
More informationMICROMECHANICS AND HOMOGENIZATION. Materials Containing Coated and Uncoated Spherical Inhomogeneities
MICROMECHANICS AND HOMOGENIZATION Materials Containing Coated and Uncoated Spherical Inhomogeneities Václav Nežerka, 2012 i Acknowledgement I would like to thank my supervisor, Jan Zeman, who supported
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More information. D CR Nomenclature D 1
. D CR Nomenclature D 1 Appendix D: CR NOMENCLATURE D 2 The notation used by different investigators working in CR formulations has not coalesced, since the topic is in flux. This Appendix identifies the
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationCVEN 5161 Advanced Mechanics of Materials I
CVEN 5161 Advanced Mechanics of Materials I Instructor: Kaspar J. Willam Revised Version of Class Notes Fall 2003 Chapter 1 Preliminaries The mathematical tools behind stress and strain are housed in Linear
More informationIntroduction to Seismology Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 12.510 Introduction to Seismology Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Stress and Strain
More informationLearning Units of Module 3
Module Learning Units of Module M. tresstrain oncepts in Three Dimension M. Introduction to Anisotropic lasticity M. Tensorial oncept and Indicial Notations M.4 Plane tress oncept Action of force (F)
More informationLecture #6: 3D Rateindependent Plasticity (cont.) Pressuredependent plasticity
Lecture #6: 3D Rateindependent Plasticity (cont.) Pressuredependent plasticity by Borja Erice and Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationModule 3: 3D Constitutive Equations Lecture 10: Constitutive Relations: Generally Anisotropy to Orthotropy. The Lecture Contains: Stress Symmetry
The Lecture Contains: Stress Symmetry Strain Symmetry Strain Energy Density Function Material Symmetry Symmetry with respect to a Plane Symmetry with respect to two Orthogonal Planes Homework References
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationA Numerical Study of Finite Element Calculations for Incompressible Materials under Applied Boundary Displacements
A Numerical Study of Finite Element Calculations for Incompressible Materials under Applied Boundary Displacements A Thesis Submitted to the College of Graduate Studies and Research in Partial Fulfillment
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationLecture 7. Properties of Materials
MIT 3.00 Fall 2002 c W.C Carter 55 Lecture 7 Properties of Materials Last Time Types of Systems and Types of Processes Division of Total Energy into Kinetic, Potential, and Internal Types of Work: Polarization
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More informationCourse No: (1 st version: for graduate students) Course Name: Continuum Mechanics Offered by: Chyanbin Hwu
Course No: (1 st version: for graduate students) Course Name: Continuum Mechanics Offered by: Chyanbin Hwu 2011. 11. 25 Contents: 1. Introduction 1.1 Basic Concepts of Continuum Mechanics 1.2 The Need
More informationElasticity in two dimensions 1
Elasticity in two dimensions 1 Elasticity in two dimensions Chapters 3 and 4 of Mechanics of the Cell, as well as its Appendix D, contain selected results for the elastic behavior of materials in two and
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationLecture 8: Tissue Mechanics
Computational Biology Group (CoBi), DBSSE, ETHZ Lecture 8: Tissue Mechanics Prof Dagmar Iber, PhD DPhil MSc Computational Biology 2015/16 7. Mai 2016 2 / 57 Contents 1 Introduction to Elastic Materials
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationChapter 16: Elastic Solids
Chapter 16: Elastic Solids Chapter 16: Elastic Solids... 366 16.1 Introduction... 367 16.2 The Elastic Strain... 368 16.2.1 The displacement vector... 368 16.2.2 The deformation gradient... 368 16.2.3
More informationLinearized theory of elasticity
Linearized theory of elasticity Arie Verhoeven averhoev@win.tue.nl CASA Seminar, May 24, 2006 Seminar: Continuum mechanics 1 Stress and stress principles Bart Nowak March 8 2 Strain and deformation Mark
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationStress/Strain. Outline. Lecture 1. Stress. Strain. Plane Stress and Plane Strain. Materials. ME EN 372 Andrew Ning
Stress/Strain Lecture 1 ME EN 372 Andrew Ning aning@byu.edu Outline Stress Strain Plane Stress and Plane Strain Materials otes and News [I had leftover time and so was also able to go through Section 3.1
More informationINVERSE ANALYSIS METHODS OF IDENTIFYING CRUSTAL CHARACTERISTICS USING GPS ARRYA DATA
Problems in Solid Mechanics A Symposium in Honor of H.D. Bui Symi, Greece, July 38, 6 INVERSE ANALYSIS METHODS OF IDENTIFYING CRUSTAL CHARACTERISTICS USING GPS ARRYA DATA M. HORI (Earthquake Research
More informationTensor Visualization. CSC 7443: Scientific Information Visualization
Tensor Visualization Tensor data A tensor is a multivariate quantity Scalar is a tensor of rank zero s = s(x,y,z) Vector is a tensor of rank one v = (v x,v y,v z ) For a symmetric tensor of rank 2, its
More informationUnit IV State of stress in Three Dimensions
Unit IV State of stress in Three Dimensions State of stress in Three Dimensions References Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationChapter 5 PlaneStress StressStrain Relations in a Global Coordinate System
Chapter 5 PlaneStress StressStrain Relations in a Global Coordinate System One of the most important characteristics of structures made of fiberreinforced materials, and one which dictates the manner
More informationModule 2 Stresses in machine elements
Module 2 Stresses in machine elements Lesson 3 Strain analysis Instructional Objectives At the end of this lesson, the student should learn Normal and shear strains. 3D strain matri. Constitutive equation;
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Uniaxial Model: StrainDriven Format of Elastoplasticity
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #3: Elastoplastic Concrete Models Uniaxial Model: StrainDriven Format of Elastoplasticity Triaxial
More informationContinuum Mechanics Fundamentals
Continuum Mechanics Fundamentals James R. Rice, notes for ES 220, 12 November 2009; corrections 9 December 2009 Conserved Quantities Let a conseved quantity have amount F per unit volume. Examples are
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationSymmetry and Properties of Crystals (MSE638) Stress and Strain Tensor
Symmetry and Properties of Crystals (MSE638) Stress and Strain Tensor Somnath Bhowmick Materials Science and Engineering, IIT Kanpur April 6, 2018 Tensile test and Hooke s Law Upto certain strain (0.75),
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationRock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth
Rock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth References: Turcotte and Schubert, Geodynamics, Sections 2.1,2.4, 2.7, 3.13.8, 6.1, 6.2, 6.8, 7.17.4. Jaeger and Cook, Fundamentals of
More informationMeasurement of deformation. Measurement of elastic force. Constitutive law. Finite element method
Deformable Bodies Deformation x p(x) Given a rest shape x and its deformed configuration p(x), how large is the internal restoring force f(p)? To answer this question, we need a way to measure deformation
More informationVYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA
VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA FAKULTA METALURGIE A MATERIÁLOVÉHO INŽENÝRSTVÍ APPLIED MECHANICS Study Support Leo Václavek Ostrava 2015 Title:Applied Mechanics Code: Author: doc. Ing.
More informationSTRESS UPDATE ALGORITHM FOR NONASSOCIATED FLOW METAL PLASTICITY
STRESS UPDATE ALGORITHM FOR NONASSOCIATED FLOW METAL PLASTICITY Mohsen Safaei 1, a, Wim De Waele 1,b 1 Laboratorium Soete, Department of Mechanical Construction and Production, Ghent University, Technologiepark
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationTheory of Plasticity. Lecture Notes
Theory of Plasticity Lecture Notes Spring 2012 Contents I Theory of Plasticity 1 1 Mechanical Theory of Plasticity 2 1.1 Field Equations for A Mechanical Theory.................... 2 1.1.1 Straindisplacement
More information16.20 HANDOUT #2 Fall, 2002 Review of General Elasticity
6.20 HANDOUT #2 Fall, 2002 Review of General Elasticity NOTATION REVIEW (e.g., for strain) Engineering Contracted Engineering Tensor Tensor ε x = ε = ε xx = ε ε y = ε 2 = ε yy = ε 22 ε z = ε 3 = ε zz =
More informationPhysics of Continuous media
Physics of Continuous media Sourendu Gupta TIFR, Mumbai, India Classical Mechanics 2012 October 26, 2012 Deformations of continuous media If a body is deformed, we say that the point which originally had
More informationMathematical Background
CHAPTER ONE Mathematical Background This book assumes a background in the fundamentals of solid mechanics and the mechanical behavior of materials, including elasticity, plasticity, and friction. A previous
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationOther state variables include the temperature, θ, and the entropy, S, which are defined below.
Chapter 3 Thermodynamics In order to complete the formulation we need to express the stress tensor T and the heatflux vector q in terms of other variables. These expressions are known as constitutive
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationNDT&E Methods: UT. VJ Technologies CAVITY INSPECTION. Nondestructive Testing & Evaluation TPU Lecture Course 2015/16.
CAVITY INSPECTION NDT&E Methods: UT VJ Technologies NDT&E Methods: UT 6. NDT&E: Introduction to Methods 6.1. Ultrasonic Testing: Basics of ElastoDynamics 6.2. Principles of Measurement 6.3. The PulseEcho
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More information3D Stress Tensors. 3D Stress Tensors, Eigenvalues and Rotations
3D Stress Tensors 3D Stress Tensors, Eigenvalues and Rotations Recall that we can think of an n x n matrix Mij as a transformation matrix that transforms a vector xi to give a new vector yj (first index
More informationNONLINEAR CONTINUUM FORMULATIONS CONTENTS
NONLINEAR CONTINUUM FORMULATIONS CONTENTS Introduction to nonlinear continuum mechanics Descriptions of motion Measures of stresses and strains Updated and Total Lagrangian formulations Continuum shell
More informationBiomechanics. Soft Tissue Biomechanics
Biomechanics crossbridges 3D myocardium ventricles circulation Image Research Machines plc R* off k n k b Ca 2+ 0 R off Ca 2+ * k on R* on g f Ca 2+ R0 on Ca 2+ g Ca 2+ A* 1 A0 1 Ca 2+ Myofilament kinetic
More informationChapter 5 Linear Elasticity
Chapter 5 Linear Elasticity 1 Introduction The simplest mechanical test consists of placing a standardized specimen with its ends in the grips of a tensile testing machine and then applying load under
More information1 Hooke s law, stiffness, and compliance
Nonquilibrium Continuum Physics TA session #5 TA: Yohai Bar Sinai 3.04.206 Linear elasticity I This TA session is the first of three at least, maybe more) in which we ll dive deep deep into linear elasticity
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More information